NOVEL ORGANIC LIGHT-EMITTING DEVICES
(B.Sci., Fudan Univ.)
A THESIS SUBMITTED
FOR THE DEGREE OF MASTER OF SCIENCE DEPARTMENT OF MATERIALS SCIENCE NATIONAL UNIVERSITY OF SINGAPORE
I would like to gratefully acknowledge those who help to make this project possible. First of all, I would like to express my deepest appreciation to my supervisor, Dr. Zhu Furong, for the enthusiastic supervision during this work. It is also my pleasure to give my sincere thanks to another two supervisors, Professor Gong Hao and Dr. Zeng Kaiyang, for their encouragements, continuous guidance and advice during the course of this work.
I am grateful to all my colleagues and friends in Institute of Materials Research &
Engineering (IMRE), for being the surrogate family during the two years I stayed there and the endless taking care thereafter. From the staff, Mr. Roshan Shrestha, Professor Osipowicz Thomas, Mr. Ong Kian Soo, Dr. Hao Xiaotao and Ms. Shen Lu are specially thanked for their kindly help and constant attention. In particular, my appreciation also goes to my two seniors, Mr. Liew Yoon Fei and Ms. Hu Jianqiao, for the numerous stimulating discussions, assistance and continuous encouragements.
In addition, I would like to acknowledge IMRE for providing a Postgraduate Research Scholarship and Top-up Award which enabled me to undertake this project.
Finally, I am forever indebted to my parents for their thoughtful understanding,
unceasing encouragement and endless moral support throughout the years.
Acknowledgments ……….……... I
Table of Contents ……….…... II
Summary …...……….. V
List of Tables ………...….…….. VII
List of Figures ……….…… VIII
Nomenclature ...………...……….... XII
List of Publications ………..…… XV
Chapter 1 Introduction ……….
1.1 General background of transparent conducting oxides ………...
1.2 Thin films of indium tin oxide ………..
1.3 Aims and objectives ………..
1.4 Organization of the thesis ……….
1 1 2 5 6
References ………... 9
Chapter 2 Basic theory and literature review ……… 13 2.1 Basic concepts and properties of ITO ……….. 13 2.2 Electrical properties of ITO ………..
2.2.1 Conduction mechanism ………
2.2.2 Carrier concentration ………
2.2.3 Carrier mobility ………
16 16 19 22 2.3 Optical properties of ITO ………..
2.3.1 Correlation between optical and electrical properties ………..
2.4 Organic light-emitting devices……….
2.4.1 Device configuration and operation ………
2.4.2 Charge injection and transport ………
2.4.3 Electroluminescence efficiency ………..
29 29 31 32
References ……….………... 35
Chapter 3 Experimental and simulation ……….………... 38
3.1 Deposition of ITO thin films ………... 38
3.2 Characterizations of ITO films ……….. 3.2.1 Electrical characterization ………... 3.2.2 Optical characterization ……….. 3.2.3 Mechanical characterization ……… 3.2.4 Structural and compositional characterization ……… 3.2.5 Surface characterization ……….. 40 40 42 44 46 48 3.3 Device fabrication and characterization. ………... 49
3.4 Thin film admittance analysis………. ……….. 3.4.1 Principle of admittance analysis ………. 3.4.2 Computer simulation ………... 50 50 52 References ……….. 55
Chapter 4 Investigation of oxygen-deficient ITO films………. 56
4.1 Electrical properties ……….. 58
4.2 Optical properties ……….. 61
4.5 Work function ………...
4.6 Surface morphology ………..
4.7 Conclusion ………
78 80 84
References ………..……… 86
Chapter 5 Application of highly oxygen-deficient ITO films ………... 89 5.1 Characterization of highly oxygen-deficient ITO films ………...
5.1.1 Electrical properties ………
5.1.2 Optical properties ………
5.1.3 Compositional properties ………
91 92 94 96 5.2 Optical destructive anode (ODA) for sunlight readable OLEDs ….……. 105 5.3 Performance of high contrast OLEDs ………... 107 5.4 Simulation of ODA-assisted OLEDs ………
5.4.1 Determination of the optical constants ………
5.4.2 Calculation of specular reflectance of OLEDs ………
5.4.3 Simulation of device contrast ………..
5.5 Conclusion ………
117 120 122
References ………..……… 124
Chapter 6 Conclusion ……….. 126
Indium tin oxide (ITO) thin films have been widely used as transparent electrodes in many optoelectronic and electro-optic devices, such as solar cells, flat panel displays and organic light-emitting devices (OLEDs), because they combine attractive properties with respect to visible transparency and electrical conductivity.
A high quality ITO film with correct stoichiometric composition is essential to its application. In spite of many investigations on ITO films, there are few studies on the estimation of the absolute oxygen concentration. In this work, the effect of hydrogen partial pressure used in the sputtering gas mixture on the properties of low-temp ITO films is discussed. The absolute oxygen concentration in the ITO films was measured by Rutherford Backscattering Spectroscopy (RBS). The correlation between the hydrogen partial pressure used in the film growth and the electrical, optical, mechanical and structural properties of ITO films also was explored. The doping efficiency of oxygen vacancies was determined by a combination of RBS and Hall measurements. Also it was found that the work function of low-temp ITO films is a function of the hydrogen partial pressure in the sputtering ambient.
The composition and the chemical state of conductive light-absorbing ITO films
were investigated using RBS and X-ray photoelectron spectroscopy (XPS). The results
reveal that a high oxygen deficiency and an increase in the atomic ratio of Sn2+
ITO films are responsible for an increase in the film absorption over the visible
wavelength. The wavelength-dependent refractive index of ITO is found to be decreased
with the oxygen deficiency.
high ambient illumination, the reflective rear electrode reflects the incident ambient light, resulting in a decreased clarity and legibility of the image. To an observer, the image visually perceived is washed out and poorly readable. It is desirable to sufficiently reduce the reflection of the ambient light from the mirror-like surface of the electrode, thereby increase the visually perceived contrast of the image.
Improving the visual contrast in OLED displays is another important issue to address with a significant technological implication. A composite optical destructive anode consisting of optically absorbing and electrically conducting oxygen-deficient ITO layer is used for high-contrast OLEDs. The OLEDs made with the optical destructive contacts exhibit a substantial reduction in the ambient light reflection from the metallic cathode, leading to an enhanced visual contrast. No manufacturing complexity, limitation of flexibility, invasive deposition process and demanding deposition requirements are involved in the device fabrication. It displayed visually superior performances with good reproducibility, while the current-voltage characteristics are comparable. Results of spectral reflectance, as well as electrical characterizations, are discussed on various OLEDs with optical destructive anodes.
The reduction of the reflectance caused by the optical destructive anode was
further investigated using optical admittance analysis. By optimizing the thickness and
the optical properties of the highly oxygen-deficient ITO layer in OLEDs, further
enhancement of the device contrast can be achieved.
Table 5.1 The compositions of ITO films measured by RBS.
Table 5.2 Elemental concentration of as-deposited ITO films prepared at different hydrogen partial pressures.
Table 5.3 Elemental concentration of Ar+
-sputtered ITO films prepared at different hydrogen partial pressures.
Table 5.4 The different optical destructive anode structures for OLEDs.
Table 5.5 SEIR and performance of OLEDs at current density of 25 mA/cm2
Figure 2.1 Schematic band structures of undoped (a) and Sn doped In2
Shaded areas denote occupied states (adapted from ).
Figure 2.2 Schematic energy band model of lightly Sn-doped In2
(adapted from ).
Figure 2.3 Energy level diagram of a two-layer OLED.
Figure 2.4 Schematic diagram showing EL process.
Figure 3.1 Multi-chamber vacuum system equipped with a magnetron sputter, a plasma pre-treatment chamber, two device process chambers and glove boxes for device characterization and testing.
Figure 3.2 Schematic diagram of four-point probe setup.
Figure 3.3 Variable angle spectroscopic ellipsometer.
Figure 3.4 Dynamic nanomechanical probe.
Figure 3.5 VG ESCALAB 220i-XL instrument.
Figure 3.6 Schematic representation of an arbitrary multilayer thin film system.
Figure 3.7 Flow chart for the computation of optical properties of OLEDs.
Figure 4.1 Dependence of resistivity (ρ), carrier mobility (µ) and concentration (N) of ITO films as a function of hydrogen partial pressure.
Figure 4.2 Optical transmittance of ITO films prepared at various hydrogen partial pressures.
Figure 4.3 Optical band gap as a function of charged carrier concentration in ITO films.
Figure 4.4 Wavelength-dependent refractive index as a function of the hydrogen partial pressure.
Figure 4.5 Wavelength-dependent extinction coefficient as a function of the
hydrogen partial pressure.
films as a function of indentation depth showing the effect of the glass substrate on the film properties measured by nano- indentation.
Figure 4.7 Variation of the elastic modulus of different ITO films on glass substrate with hydrogen partial pressure in the sputtering gas mixture.
Figure 4.8 Hardness of ITO films on glass substrates as a function of hydrogen partial pressure in the sputtering ambient.
Figure 4.9 A typical RBS spectrum of ITO film on glass substrate.
Figure 4.10 Oxygen content in ITO films measured by RBS, as a function of hydrogen partial pressure.
Figure 4.11 Measured carrier concentration as a function of the absolute oxygen concentration in the films.
Figure 4.12 The work function measured for ITO films prepared at different hydrogen partial pressures.
Figure 4.13 AFM images measured for ITO films prepared at different hydrogen partial pressures of (a) 0, (b) 1.1×10-3
Pa, (c) 2.0×10-3
Pa, (d) 2.6×10-3
Pa and (e) 4.0×10-3
Figure 4.14 The variation of ITO surface roughness as a function of hydrogen partial pressure.
Figure 5.1 Variation of the electrical resistivity with the hydrogen partial pressure in the sputtering ambient.
Figure 5.2 Transmittance of ITO films prepared at various hydrogen partial pressures.
Figure 5.3 RBS spectra of ITO films prepared at different hydrogen partial pressures in the sputtering ambient.
Figure 5.4 In 3d XPS spectra of as-deposited ITO films prepared at different hydrogen partial pressures.
Figure 5.5 In 3d XPS spectra of Ar+
-sputtered ITO films prepared at different
hydrogen partial pressures.
Figure 5.7 Sn 3d5/2
XPS spectra of Ar+
-sputtered ITO films prepared at various hydrogen partial pressures.
Figure 5.8 O 1s XPS spectra of as-deposited ITO films prepared at various hydrogen partial pressures.
Figure 5.9 O 1s XPS spectra of Ar+
-sputtered ITO films prepared at various hydrogen partial pressures.
Figure 5.10 A cross sectional view of the ODA-assisted OLEDs.
Figure 5.11 Current-voltage characteristics of a conventional OLED and the OLEDs made with optical destructive anodes.
Figure 5.12 Luminance-current characteristics of the OLEDs made with optical destructive anodes and a conventional OLED.
Figure 5.13 Wavelength-dependent reflectance spectra measured for a control device and high contrast OLEDs made with different ODAs varied in (a) layer thickness and (b) hydrogen partial pressure used for the ODITO layer.
Figure 5.14 Illumination showing the light traveling routes for both internal emitted light of conventional OLEDs and ambient light.
Figure 5.15 Optical images of (a) a control device, (b) an ODA-assisted device.
Figure 5.16 Refractive index and extinction coefficient extracted for NPB layer with a thickness of about 50 nm.
Figure 5.17 Refractive index and extinction coefficient extracted for Alq3
layer with a thickness of about 40 nm.
Figure 5.18 Wavelength-dependent refractive index and extinction coefficient of ITO films as a function of the hydrogen partial pressure.
Figure 5.19 Calculated and measured spectral reflectance of the device with a configuration of glass/ODITO(300nm)/ITO(130nm)/NPB(60nm)/
Figure 5.20 Measured and calculated integrated spectral reflectance, over the
wavelength range of 400 to 700nm, of ODA-assisted OLEDs as a
function of the hydrogen partial pressure.
specular reflectance of ODA-assisted OLEDs, (b) to calculate the visually perceived luminance of ODA-assisted OLEDs.
Figure 5.22 Normalized /R of OLEDs with ODAs prepared at different hydrogen partial pressures as a function of the ODITO layer thickness.
AFM Atomic force microscopy
Tris-(8-hydroxyquinoline) aluminum BM Burstein-Moss
CSM Continuous stiffness measurement DCM Dynamic contact module
EPMA Electron probe microanalysis HOMO Highest occupied molecular orbital HTL Hole transporting layer
ITO Indium tin oxide
J-V-L Current density-voltage-luminance LUMO Lowest unoccupied molecular orbital
NPB N, N'-di(naphthalene-1-yl)-N, N'-diphenylbenzidine OLEDs Organic light-emitting devices
PLD Pulsed laser deposition
PLEDs Polymer light-emitting devices
RBS Rutherford backscattering spectroscopy rf Radio frequency
RMS Root mean square
SEIR Sun/eye-integrated reflectance
TOLEDs Top-emitting organic light-emitting devices
UPS Ultraviolet photoelectron spectroscopy VASE Variable angle spectroscopic ellipsometry VRH Variable range hopping
XPS X-ray photoelectron spectroscopy
A(λ) Wavelength dependent absorbance E Elastic modulus
Conduction band Ef
Fermi energy level Eg
Direct optical band gap Eopt
Optical band gap
k Extinction coefficient
m* Effective mass of the electron N Carrier concentration
n Refractive index P Porosity
Integrated normalized reflectance
T(λ) Wavelength dependent transmittance α Absorption coefficient
µ Hall mobility
h ν Photon energy
Frequency of electromagnetic oscillations
η Doping efficiency
1. W. W. Zheng, F. R. Zhu, H. Gong, T. Osipowicz, Dependence of the hydrogen partial pressure in the sputtering ambient on the optical and electrical properties of low temperature indium tin oxide thin films, to be submitted to J. Appl. Phys.
2. W. W. Zheng, Y. F. Liew, F. R. Zhu, Optical destructive anode for sunlight readable organic light-emitting devices, to be submitted to Appl. Phys. Lett.
3. W. W. Zheng, Y. F. Liew, F. R. Zhu, Low-reflectance anode for contrast enhancement
of organic light-emitting devices, to be submitted to Adv. Mater.
CHATPER 1 INTRODUCTION
1.1 General background of transparent conducting oxides
Thin films of transparent conducting oxides (TCOs) are highly transparent in the visible region and reflective in the infrared region with nearly metallic like conductivity.
TCO thin films have been widely used in optoelectronic devices due to their unique electrical and optical properties. The cadmium oxide (CdO) is the first reported TCO that possesses both transparent and conducting properties . Thin films of metals (~100-200 Å) such as Au, Ag, Cu, Fe also exhibit a high electrical conductivity and a relatively high optical transmittance, but the thin metallic films, in general, are not very stable in air and have limitations in device applications. Compared with the metallic thin films, TCO films are particularly more useful because of their superior chemical stability and hardness.
It is now known that thin films of non-stoichiometric or doped metal oxide such as indium oxide, tin oxide, zinc oxide and cadmium stannate exhibit high transparency and nearly metallic like conductivity [2-4]. Generally, TCO films are n-type and highly degenerated wide-gap semiconductors with an optical band gap range of 3~4.5 eV [2, 3].
Recently much effort has been focused on exploring p-type TCOs for novel all-oxide transparent or semitransparent opto-electronic devices. Kawazoe et al  reported a p- type oxide semiconductor CuAlO2
. Thus it shows promise of the potential applications of transparent p-n junction by combining both n-type and p-type TCO films.
Many new materials and manufacturing techniques have been developed to satisfy
stringent technological requirements. The required quality of the films increases with the
boosting sophistication of the applications. Accounting for the unique combined electrical and optical properties, TCO films have found a variety of applications.
Coatings of In2
and ITO are widely used in many applications including heat mirrors , energy saving windows , transparent electrodes for displays [8-14], transparent electrodes in solar cells [15-22], gas sensors [23-28], corrosion-resistant coatings [29-32]. The selection of a suitable material for a specific application depends on its electrical, optical and mechanical properties as well as chemical stability.
In addition to the above applications, TCOs have also been used as buffer layers in superconducting thin films , gate electrodes in MOS capacitors , active elements in transparent thermocouples , electrodes in ferroelectric films , optical memory materials in optical recording devices  and varistors . ITO film is resistant to laser damage and is a potential candidate for use in Pockel’s cell .
1.2 Thin films of indium tin oxide
Among the existing TCOs, ITO is one of the most important and it is widely used TCO materials due to its superior characteristics. In view of its practical importance, a great deal of basic research and development has been carried out for better understanding the electrical and optical properties of ITO films.
The properties of ITO films are strongly dependent on the process conditions and
deposition techniques. Much effort has been carried out to understand the physical
phenomena in ITO and the limitations that are hampered by the variety of preparation
methods. Vossen , Jarzebski , Manifacier , Dawar and Joshi , and Chopra
et al  have reviewed the different thin film preparation techniques, the properties of ITO and their importance in thin film technology. Hamberg and Grangvist summarized the basic optical properties of ITO and discussed their potential for applications as the energy saving windows .
Various manufacturing techniques have been developed to meet both economic and technological demands. Thermal evaporation deposition , magnetron sputtering [46, 47], electron beam evaporation , spray pyrolysis , chemical vapour deposition , dip-coating techniques [51, 52], and pulsed laser deposition [53, 54] are some of the preparation methods currently used for different applications. In particular, sputtering is one of the most versatile techniques used for the fabrication of high quality ITO films. Compared with other deposition techniques, the sputtering process produces films with higher purity, better-controlled composition, greater adhesive strength and better film uniformity.
The development of organic light-emitting devices, this last decade, boosted the
research on ITO films. It is shown that both surface and bulk properties of ITO play an
important role in determining the performance of OLED. Much work has been focused
on films deposited onto glass substrates or other rigid substrates. However, glass
substrates are unsuitable for certain applications such as electronic maps, smart cards, and
portable computers where flexibility, weight, and/or safety issues are important. Glass is
very brittle and difficult to be deformed or used in flexible devices. These disadvantages
can be overcome using flexible plastic substrates which are robust, lightweight, and cost
effective. For these reasons, flexible plastic substrates have been used in passive and
active matrix displays  such as liquid crystal displays and polymeric and molecular organic light-emitting devices [56-59]. Future displays will essentially be based on active matrix displays. The complexity of the addressing circuitry for these displays continuously increases and often includes three or four thin film transistors (TFT) at each pixel. This makes the substrate pretty opaque and high-resolution displays could only be achieved using top-emitting OLED architecture where ITO is required to form on the top of the active organic layers. Such geometry could also be of paramount interest for OLED microdisplays that are built on silicon thin film transistors. Another device requiring ITO-on-top electrode is the transparent OLEDs first reported by the Princeton group . The challenge for above-mentioned devices relies on the capability of deposition high quality ITO under soft enough conditions so as to avoid any degradation of the underlying plastic substrates or organic materials during ITO deposition. High performance ITO films are usually deposited at a substrate temperature over 200 ˚C and/or required a postdeposition annealing process to improve the overall ITO quality.
However, plastic substrates or organic materials are not compatible to high substrate temperature as the glass transition temperature of the organic layers or the plastic substrates is much lower. Therefore it is essential and particularly important to develop a technique to produce high quality ITO at a low processing temperature.
It was reported by Hamberg et al that ITO prepared at a low temperature and
oxygen-deficient ambient are absorbing and somewhat conductive . The blackening of
ITO films is observed during deposition of ITO films [61-64] and/or the subsequent
sputtering of dielectric films on ITO-coated substrates [65-67]. ITO is essentially In2
based material that is doped with Sn to improve electrical conductivity. The presence of
metal indium in ITO/silicon oxide/Si junction solar sells was one of the main factors causing dark ITO that deteriorate the device performance. Wu and Chiou  and Matsuoka et al  argued that the reduction of SnO2
in ITO films resulted in the blackening of ITO. Fan and Goodenough  considered that the darkening of ITO was due to the formation of a second phase in the bulk of the films. While the mechanism for the blackening of ITO films is still not clear, the stoichiometry of the oxide film seems to be an important factor in both optical transparency and electrical conductivity.
For conventional OLEDs, high transparency of ITO layer is desirable. To increase efficiency and reduce driving voltage, the low work function metal cathodes for OLEDs are utilized, usually resulting in high reflection [14, 68]. In high ambient illumination, the reflective metallic electrode reflects the incident ambient light, resulting in a decrease in contrast of the visual image. To an observer, image visually perceived is washed out and poorly legible. In many applications, particularly in outdoors or in brightly illuminated environment, visual contrast may be more important than the brightness of the image.
The conductive light-absorbing ITO shows the potential to serve as a non-reflective layer in the device to enhance the device contrast.
1.3 Aims and objectives
This research aimed at providing systematic studies of oxygen deficient ITO films
prepared at a low processing temperature using rf magnetron sputtering. The potential
applications, particularly in novel OLEDs, have been explored. In addition, this work also
identified the important areas for future experimental and theoretical studies. The primary
objectives of this research were:
1. To develop a process to deposit optimal ITO at a low processing temperature suitable for high contrast OLEDs;
2. To better understand the optical, electrical, mechanical and structural properties of oxygen-deficient ITO;
3. To study the correlation between electrical and optical properties of amorphous ITO;
4. To investigate the doping efficiency of oxygen vacancies in amorphous ITO;
5. To prepare and characterize highly oxygen-deficient ITO;
6. To fabricate and characterize sunlight readable OLEDs with a composite optical destructive anode;
7. To design and optimize sunlight readable OLEDs using optical admittance analysis.
1.4 Organization of the thesis
In Chapter 2, the background and the relevant literature survey of ITO are presented. The basic concepts and the fundamental properties of ITO are discussed. The growth techniques employed for the preparation of ITO thin films are summarized. The principle, device architecture and fabrication of OLEDs are reviewed. The recent progresses made in high contrast OLEDs are also discussed.
In Chapter 3, the experimental procedures including the growth of ITO film at a
low processing temperature and in an oxygen-deficient ambient are described. The
characterization methods with respected to the optical, electrical, mechanical and
structural properties of ITO are presented. The design, fabrication and characterization of
OLEDs are addressed. The principles of computer simulation using optical admittance analysis, as well as the simulation setup, are briefly introduced.
In Chapter 4, the findings concerning the properties of low-temperature ITO prepared at oxygen–deficient ambient are presented. The effect of the hydrogen partial pressure in the processing gas mixture on the electrical, optical, mechanical and structural properties of ITO films is investigated. Rutherford backscattering spectroscopy (RBS) was utilized to determine the doping efficiency of the oxygen vacancy in ITO films. It is found that there are more than ten times as many oxygen vacancies as they would be expected from the carrier concentration measurements. It is therefore clear from this work that the doping mechanism of a low-temperature ITO is more complex than the usual picture of every oxygen vacancy producing two free electrons. The correlation between the hydrogen partial pressure in the sputtering ambient and the electrical and optical properties of low-temperature ITO is discussed. This work also revealed that the work function of the ITO films can be adjusted by varying hydrogen partial pressure during the film deposition.
In Chapter 5, the principle of sunlight readable OLEDs fabricated with an optical
destructive anode (ODA) is discussed. This novel anode incorporates a conductive light-
absorbing oxygen-deficient ITO layer and a transparent ITO layer. The sunlight readable
OLEDs demonstrate a sun/eye-integrated reflectance (SEIR) of 13%, which is about 5
times lower than that of the standard device, while the current-voltage characteristics are
comparable. RBS and X-ray photoelectron spectroscopy (XPS) were used to investigate
the composition and the chemical state of the conductive light-absorbing layers. The
results show that a high oxygen-deficient ITO had a higher atomic ratio of Sn2+
in the film compared to the transparent ITO. The blackening of the ITO films is associated with the nature of high Sn2+
in the film. A significant decrease in the wavelength- dependent refractive index in a highly oxygen-deficient ITO was determined by the variable angle spectroscopic ellipsometry (VASE) over the visible light spectrum. The reduction of the specular reflectance of OLED, which is caused by the optical destructive anode, was further analyzed by computer simulation using admittance analysis. The simulated specular reflectance of sunlight readable OLEDs agreed well with the measured specular reflectance.
In Chapter 6, the research findings and the important results of this work are
summarized. In addition, future work on optimization of sunlight readable OLEDs and
improvement of the legibility of the devices is proposed.
1. K. Bedeker, Ann. Phys. 1907, 22, 749.
2. L. J. Meng, M. P. Dos Santos, Thin Solid Films 1998, 322, 56.
3. M. Bender, W. Seelig, C. Daube, H. Frankenberger, B. Ocker, J. Stollenwrek, Thin Solid Films 1998, 326, 72.
4. J. Nishino, T. Kawarada, S. Ohshio, H. Saitoh, K. Maruyama, K. Kamata, J.
Mater. Sci. Lett. 1997, 16, 629.
5. H. Kawazoe, M. Yasukawa, H. Hyodo, M. Kurita, H. Yanagi, H. Hosono, Nature 1997, 389, 939.
6. H. Dewall, F. Simonis, Thin Solid Films 1981, 77, 253.
7. I. Hamberg, C. G. Granqvist, J. Appl. Phys. 1986, 60(11), R123.
8. R. Latz, K. Michael, M. Scherer, Japan. J. Appl. Phys. 1991, 30, L149.
9. N. Kuck, K. Lieberman, A. Lewis, A. Vecht, Appl. Phys. Lett. 1992, 61, 139.
10. N. Miura, T. Ishikawa, T. Sasaki, T. Oka, H. Ohata, H. Matsumoto, R. Nakano, Japan. J. Appl. Phys. 1992, 31, L46.
11. M. Hagerott, H. Jeon, A. V. Nurmikko, W. Gunshor, Appl. Phys. Lett. 1992, 60, 2825.
12. Y. Chubachi, K. Aoyama, Japan. J. Appl. Phys. 1991, 30, 1442.
13. Y. Hamada, C. Adachi, T. Tsutsui, S. Saito, Japan. J. Appl. Phys. 1992, 31, 1812.
14. C. W. Tang, S. A. Vanslyke, Appl. Phys. Lett. 1987, 51, 913.
15. N. Croitoru, E. Bannett, Thin Solid Films 1981, 82, 235.
16. R. Singh, M. A. Green, K. Rajkanan, Solar Cells 1981, 3, 95.
17. J. Shewchun, J. Dubow, A. Myszkowski, R. Singh, J. Appl. Phys. 1978, 49, 855.
18. J. Shewchun, D. Burk, M. B. Spitzer, IEEE Trans. Electron. Devices 1980, 27, 705.
19. A. K. Ghosh, C. Fishman, T. Feng, J. Appl. Phys. 1978, 49, 3490.
20. S. Major, S. Kumar, M. Bhatnagar, K. L. Chopra, Appl. Phys. Lett. 1986, 49, 394.
21. S. Ray, J. Dutta, A. K. Barua, S. K. Deb, Thin Solid Films 1991, 199, 201.
22. S. K. Das, G. C. Morris, J. Appl. Phys. 1993, 73, 782.
23. S. S. Sharma, K. Nomura, Y. Ujihira, J. Appl. Phys. 1992, 71, 2000.
24. H. Pink, L. Treitinger, L. Vite, Japan. J. Appl. Phys. 1980, 19, 513.
25. Y. K. Fang, F. Y. Chen. J. D. Hwang, B. C. Fang, J. R. Chen, Appl. Phys. Lett.
1993, 62, 490.
26. S. C. Chang, IEEE Trans. Electron. Devices 1979, 26, 1875.
27. H. Nanto, H. Sokooshi, T. Kawai, T. Usuda, J. Mater. Sci. Lett. 1992, 11, 235.
28. K. Fukui, Sens. Actuators B 1991, 5, 27.
29. A. Roos, P. Hedenqvist, Appl. Phys. Lett. 1991, 59, 25.
30. A. Roos, P. Hedenqvist, Proc. SPIE 1990, 1275, 148.
31. A. Roos, Thin Solid Films 1991, 203, 41.
32. V. J. Novotny, A. S. Kao, IEEE Trans. Mag. 1990, 26, 2449.
33. B. J. Kellett, A. Gauzzi, J. H. James, B. Dwir, D. Paveuna, F. K. Reinhart, Appl.
Phys. Lett. 1990, 57, 2588.
34. C. H. Weijtens, IEEE Trans. Electron. Devices 1992, 39, 1889.
35. K. G. Kreider, Sens. Actuators A 1992, 34, 95.
36. C. W. Kwok, D. P. Vijay, S. B. Desu, N. R. Parikh, E. A. Hill, Integrated Ferroelectrics 1993, 3, 121.
37. M. C. de Andrade, S. Moehlecke, Appl. Phys. A 1994, 58, 503.
38. R. D. Gould, A. K. Hassan, F. S. Mahmood, Int. Electron. 1994, 76, 895.
39. W. T. Pawlewicz, J. B. Mann, W. H. Lowdermilk, Milam, Appl. Phys. Lett. 1979, 34, 196.
40. J. L. Vossen, Thin Solid Films 1977, 9, 1.
41. Z. M. Jarzebski, Phys. Status Solidi A 1982, 71, 13.
42. J. C. Manifacier, Thin Solid Films 1982, 90, 297.
43. A. L. Dawar, J. C. Joshi, J. Mater. Sci. 1984, 19, 1.
44. K. L. Chopra, S. Major, D. K. Pandya, Thin Solid Films 1983, 102, 1.
45. A. Salehi, Thin Solid Films 1998, 324, 214.
46. K. Zhang, F. Zhu, C. H. A. Huan, A. T. S. Wee, J. Appl. Phys. 1999, 86, 974.
47. K. Zhang, F. Zhu, C. H. A. Huan, A. T. S. Wee, T. Osipowicz, Surf. Interface Anal. 1999, 28, 271.
48. J. K. Sheu, Y. K. Su, G. C. Chi, M. J. Jou, C. M. Chang, Appl. Phys. Lett. 1999, 72, 3317.
49. S. Major, K. L. Chopra, Sol. Energy Mater. 1988, 17, 319.
50. J. Hu, R. G. Gordon, J. Appl. Phys. 1992, 72, 5381.
51. Y. Takahashi, S. Okada, R. B. H. Tahar, K. Nakano, T. Ban, Y. Ohya, J. Non-Cry.
Solids 1997, 218, 129.
52. K. Nishio, T. Sei, T. Tsuchiya, J. Materials Sci. 1996, 31, 1761.
53. H. S. Kwok, X. W. Sun, D. H. Kim, Thin Solid Films 1998, 335, 299.
54. H. Kim, A. Piqué, J. S. Horwitz, H. Mattoussi, H. Murata, Z. H. Kafafi, D. B.
Chrisey, Appl. Phys. Lett. 1999, 74, 3444.
55. N. D. Young, R. M. Bunn, R. W. Wilks, D. J. McCulloch, S. C. Deane, M. J.
Edwards, G. Harkin, A. D. Pearson, J. Soc. Inf. Disp. 1997, 5/3, 275.
56. G. Gustafsson, Y. Cao, G. M. Treacy, F. Klavetter, N. Colaneri, A. J. Heeger, Nature 1992, 357, 477.
57. G. Gu, P. E. Burrows, S. R. Forrest, Opt. Lett. 1997, 22, 172.
58. G. M. Daly, H. Murata, C. M. Merritt, Z. H. Kafafi, H. Inada, Y. Shirota, Mater.
Res. Soc. Symp. Proc. 1998, 488, 33.
59. Y. He, J. Kanicki, Appl. Phys. Lett. 2000, 76, 661.
60. G. Pathasarathy, P. E. Burrows, S. R. Forrest, Appl. Phys. Lett. 1998, 72, 2138.
61. H. Kobayashi, T. Ishida, K. Nakamura, Y. Nakato, H. Tsubomura, J. Appl. Phys.
1992, 72, 5288.
62. W. F. Wu and B. S. Chiou, Thin Solid Films 1994, 247, 201.
63. J. C. C. Fan and J. B. Goodenough, J. Appl. Phys. 1977, 48, 3524.
64. W. F. Wu, B. S. Chiou, S. T. Hsieh, Semicond. Sci. Technol. 1994, 9, 1242.
65. T. Matsuoka, J. Kuwata, Y. Fujita, A. Abe, Japan. J. Appl. Phys. 1998, 27, L1199.
66. Y. Chubachi, K. Aoyama, Japan. J. Appl. Phys. 1991, 30, 1442.
67. M. P. R. Panicker, W. F. Essinger, J. Electrochem. Soc. 1981, 128, 1943.
68. T. Wakimoto, Y. Fukuda, K. Nagayama, A. Yokoi, H. Nakada, M. Tsuchida,
IEEE Trans. Electron Devices 1997, 44, 1245.
CHATPER 2 BASIC THEORY AND LITERATURE REVIEW
2.1 Basic concepts and properties of ITO
crystallizes with a bixbyite, C-type cubic, rare earth sesquioxide crystal structure with space group . Each indium atom is surrounded by six oxygen atoms at the corner of a distorted cube, with two vacancies at the two unoccupied corners.
The lattice parameter of In
Ia 3 Th
is 10.117 Å. The unit cell contains 80 atoms and as such, the structure is highly complicated. However, Hamberg and Granqvist  and Fan and Goodenough  have proposed a simple band structure to explain the conduction mechanism in In2
According to Hamberg and Granqvist , the band structure of In2
, shown in Fig 2.1 (a), has parabolic bands characterized by effective mass of the free electrons for the conduction band and for the valence band. The direct band- gap denoted by
is 3.75 eV. The dispersions for the valence and conduction bands are given as:
E ( ) 2
E k k
E ( ) 2
2 2 0
h , (2.2)
where k is the wave vector. Superscript 0 denotes unperturbed bands.
Indium tin oxide retains a crystal structure of undoped-bulk In2
However the lattice constant values are usually higher than those in undoped-bulk In2
incorporation of tin ions in interstitial positions. The ITO films, in general, exhibit a strong (1 1 1) or (1 0 0) preferred orientation depending on the deposition conditions.
The properties of ITO can be understood by superimposing the effect of tin doping on the host lattice of In2
As already mentioned, the crystal structure of In2
is highly complicated and as such the calculations of ITO band structure have not been made. Hamberg and Granqvist  have assumed an ITO band structure, shown in Fig.
2.1 (b). In the case of ITO, A partial filling of the conduction band as well as shifts in the energy of the bands relative to their locations in In2
takes place as indicated in Fig. 2.1.
As a result of doping, there is a blocking of the lowest states in the conduction band and hence a widening of Eg,
but at the same time electron-electron and electron-impurity scattering tend to decrease the gap. This is illustrated as Eg0
> W in Fig. 2.1, where W is
Fig. 2.1 Schematic band structures of undoped (a) and Sn doped In2
(b). Shaded areas denote occupied states (adapted from ).
v v v
E k E
) h (
2 ) (
g c c
m E k k E
c c c
E k E
) h (
m k k E ( )
2 2 0
the energy difference between the top of the valence band and bottom of the conduction band in ITO. This effect can be described by replacing the dispersion of unperturbed bands, equations (2.1) and (2.2), by the following relations:
k E k k
E ( )0
( ) h , (2.3)
k E k k
E ( )0
( ) h , (2.4)
where h ∑v
and h ∑c
are self-energies due to electron-electron and electron-impurity scattering.
are self-energies due to electron-electron and electron-impurity scattering.
~0.03 eV Sn3+
Fig. 2.2 Schematic energy band model of lightly Sn-doped In2
(adapted from ).
is usually oxygen deficient. The oxygen vacancies usually give rise to a shallow donor level just below the conduction band. In the case of ITO, Sn: 5s level is stabilized just below Ec
. Unlike oxygen vacancies Vo
, a two-electron donor level, Sn: 5s level is a one-electron donor level. In ITO films, Vo
and Sn: 5s levels co-exist and both contribute conduction electrons as shown in Fig. 2.2. When a small amount of Sn is added in In2
the Sn enters substitutionally in the cation sublattice. Hence, the Sn4+
and acting as an n-type donor. The new material can be represented as In2- y
2.2 Electrical properties
Electrical conductivity (σ) depends on the concentration (N) and mobility (µ) of relevant free carrier as follows:
σ = Nµe, (2.5)
where e is the electron charge. In order to obtain films with high conductivity, high carrier concentration and mobility should be simultaneously realized. The electrical properties of the TCOs depend critically upon the oxidation state of the metal component (stoichiometry of the oxide) and on the nature and quantity of impurities incorporated in the films.
2.2.1 Conduction mechanism
has the cubic bixbyite structure in which O2-
ions occupy, in an ordered
matter, three-fourths of the tetrahedral interstices of a face-centered-cubic In3+
. Indium tin oxide should have a filled O2-
: 2p valence band that is primarily oxygen 2p in character . The In: 3d core lies below the valence band edge Ev
. The conduction band is the metal-5s band with an edge Ec
about 3.5 eV above Ev
[5, 6]. The next higher band is the metal-5p band. Generally, In2
lacks stoichiometry due to oxygen vacancies Vo
. At high Vo
concentration, a Vo
impurity band forms and overlaps
at the bottom of the conduction band producing a degenerate semiconductor. The oxygen vacancies act as doubly ionized donors and contribute at a maximum two electrons to the electrical conductivity. Tin acts as a cationic dopant in the In
lattice and substitutes the indium, providing an electron to the conduction band.
The defect structure of In2
has been studied by De Wit et al [7, 8]. Oxygen vacancies are considered as the predominant point defects in In2
according to the following reaction:
+ 6e′ + 2
denotes doubly charged oxygen vacancies and e′ denotes electrons which are needed for charge neutrality on the macroscopic scale.
Frank and Kostlin  have suggested that oxygen-deficient In2
can be represented as In2
′, where x is normally less than 0.01.
There are three types of defects have been proposed for ITO films with high Sn
doping concentration. They are an ionized ( Sn2⋅
) complex involving an interstitial O
atom loosely bound to two Sn atoms, a nonionizable ( Sn2
complex composed of two nearby Sn atoms which strongly bind three closest O atoms together with an additional O atoms, and a ( Sn2⋅
associate . However these three defects are expected to play a marginal role.
In amorphous materials, the hopping process is the most dominant conduction mechanism. The conductivity due to hopping process can be expressed as:
] ) ( exp[0
2 / 1
σ , (2.7)
where the value of x depends on the dimentionality and nature of the hopping process.
When conduction is three dimentional, variable range hopping (VRH) gives = 0.25 for constant density of states and = 0.5 for a parabolic density of states .
In amorphous materials, VRH conduction occurs at temperatures at which the photons do not have sufficient energy for transfer to a nearest neighbor atom, and the charge carriers hop from a neutral atom to another neutral atom situated at the same energy level, which can be many inter-atomic distance away. The most commonly used model for VRH is due to Mott , which is based on a number of assumptions, e.g. (i) energy independent of the density of states, (ii) neglect of correlation effects in the tunneling process, (iii) omission of multiphoton process, (iv) neglect of electron-photon interaction. According to Mott’s theory:
] ) ( exp[0 1/4
2 / 1
σ , (2.8)
2 / 1 2
8 ) [ (
σ = , (2.9)
E T kN λ α
= , (2.10)
4 / 1
) ( 8 [ 9
N R R
= π , (2.11)
) ( 4
N W R
= π , (2.12)
where N ( EF
) is the density of states near the Fermi level, λc
is a dimentionless constant (≈ 18), ν is a frequency factor taken here as the Debye frequency (≈ 3.3×10ph 12
Hz), α is the decay constant of the wave function of the localized states near the Fermi level, R is the mean hopping distance and W is the hopping energy.
2.2.2 Carrier concentration
Most of the efforts made to improve the conductivity of the material have been focused on increasing the effective number of free carriers (N) via doping. Although this method had some success, it is self-limiting. As the dopant atoms occupy random sites in the host lattice, the process of doping certainly impairs the mobility while increasing N.
Hence, obtaining the lowest possible resistivity is a trade-off between carrier
concentration and electron mobility. The following relation deduced by Johnson and
Lark-Horovitz  for a complete degeneracy, µ = (4e/h) (π/3)1/3
= 9.816 × 1014
), shows that the mobility ( µ ) and carrier concentration (N) are no longer
independent but are governed by a rule µ = ∝ N−2/3
. Furthermore, at high dopant
expected assuming that every soluble tin atom contributes one free electron. This implies that a portion of the tin remains electrically inactive. Assuming that the higher the tin content the more probable the tin ions occupy the nearest-neighboring anion sites, Köstlin, Jost, and Lem  presented two arguments to elucidate the annihilation effect of two Sn cations.
(1) The additional Sn anion changes its valence from 4+ to 2+, forming a neutral complex of Sn2+
with respect to the normal matrix.
(2) The tin pair substituting two neighboring indium atoms strongly binds additional oxygen, forming a neutral complex that consists of the two Sn4+
ions and the additional oxygen, that is, Sn2
Based on Mössbauer spectra which did not confirm the existence of divalent Sn anions at any tin concentration, the second possibility seems to be the more probable.
Meng et al  supported this view by performing an X-ray photoelectron spectroscopy (XPS) measurement. They showed that the increase in carrier concentration due to a high temperature annealing is not ascribed to the transition of SnO to SnO2
Two more models are considered in literature [15, 16] for the compensation of tin donor:
(1) Anion interstitial model: completely filled cation sublattice with an excess of δ/2
) on a quasianion sublattice neutralizing the δ ionized tin donors,
(2) Cation vacancy model: creation of δ/3 cation vacancies (VIn
) to preserve electrical neutrality, formally, In2-4δ/3
Frank and Köstlin  rejected the second model because they did not notice any increase in film thickness during oxidation as expected. On the basis of the first model they proposed the formation of the following neutral defects.
"): Two Sn4+
ions which are not on nearest-neighbor positions loosely bound to an interstitial oxygen anion. This interstitial defect dissociates on annealing under reducing conditions: Sn2
" ⇄ 2Sn + 2e−
: Two nearest-neighbor Sn4+
ions bound to three nearest neighbors on regular anion sites and an additional interstitial oxygen ion on nearest quasianion site. This neutral defect was previously discussed .
: Associate of the two above mentioned defects.
Other macroscopic factors controlling the doping efficiency were also postulated.
According to Mizuhashi , the high impurity level results in the distorted crystal lattice
so that it can no longer be effective either in generating Sn4+
ions on substitutional sites
or in generating oxygen vacancies. Excessive disorder in the form of an intergranular
amorphous phase is also observed . Na et al  studied the way in which excessive
tin oxide affects the properties of ITO films. They observed continuous SnO2
along the grain boundaries. Ryabova et al  deposited ITO films by the pyrolysis
method. The film homogeneity was improved after annealing as a result of the diffusion
of tin atoms in the In2
matrix. As a consequence, the lattice disorder was decreased and hence the mobility in the annealed films increased. Recently, Haynes and Shigesato 
showed that In+
implantation into ITO films, prepared by conventional electron beam evaporation, increases the carrier concentration by simultaneously generating excess vacancies (displacement of atoms from lattice sites during collisions) and stabilizing the excess oxygen vacancies (introduction of cations). It was also reported  that implantation of H+
improved the resistivity of sputtered ITO films due to the creation of oxygen vacancies.
2.2.3 Carrier mobility
The carrier mobility of the carriers in ITO films is strongly dependent on the particular structure of In2
[6, 24] and the modification of the network . As a consequence, there is a strong scattering effect on free carriers. Thereby the mobility is considerably lowered. There are many sources of electron scattering which may influence the electrical and optical properties of the ITO films. Scattering by grain boundaries and acoustical photons  apparently play a subordinate role since in the majority of the cases the mean free path length of electron is smaller than the crystallite size . Nevertheless, grain boundary scattering [28-32] is sometimes, postulated in ITO films with small crystallite size as an important factor that contributes to the decrease in the mobility. In some cases, domain (coalescences of ordered grains) boundaries [33, 34] are assumed to affect the mobility rather than the grain boundaries.
Domain boundaries of an ITO film might act as a barrier height [35-37] which obstructs
the motion of conductive electrons in the conduction band. Therefore, an increase in the
Hall mobility might be expected in ITO films with larger domains. In ITO films with
good crystallinity, electron scattering by dislocations and precipitation  is expected to be of little importance.
It was pointed out that scattering of the conduction electrons by neutral and ionized impurity centers can dramatically affect the conductivity of semiconductors.
Based on the work of Massey and Moiseiwitch , Erginsoy  evaluated the resistivity due to neutral impurities which should be taken into account particularly in semiconductors with small degrees of ionization. The contribution to the resistivity by ionized impurities was calculated by Conwell and Weisskopf . Later, Dingle 
derived a more refined description of the scattering effect. On the basis of the above mentioned theory, the following relations [17, 42-47] have been used to describe the effect of neutral and charged scattering centers on the mobility of degenerate semiconductors:
= ( m*
) /( 20 ε0
) , (2.13)
] ) ( /[
] ) ( 24
[3 0 r 2 3 3 *2 2 I
π ε ε h n e m g x z N
µ = . (2.14)
The screening function g(x) is given by
4 / 1 ( ) / 4 1 ln(
( x = + x − + x−
g , (2.15)
where can be expressed as: x
3 ( 4
h2 5 1/3
x = πε εr
π , (2.16)
where is the carrier concentration, n z is the charge of the ionized centers, ε0
is the permittivity of free space, m*
is the effective mass of the free electrons, and εr
is the low-frequency relative permittivity. For ITO, the m*
values can be taken as 0.3 and 9 [2, 43], respectively.
are the mobilities due to neutral and ionized scattering impurities, and N and are the density of neutral and ionized scattering centers, respectively. The total mobility
can be taken as the reciprocal sum of µN
1 = + . (2.17)
2.3 Optical properties
The thin films of transparent conducting oxides, in general, are electrically conductive and optically transparent over the visible wavelength range, but are reflective to the thermal infrared radiation. For longe wavelength region, the high reflectivity is attributed to a high free electron concentration in TCOs. Over the short wavelength region, the absorption is attributed to the fundamental band-gap.
2.3.1 Correlation between optical and electrical properties
The real and imaginary parts of the dielectric constants ( ε = ε1
+ i ε2
) are related to the optical constant ( N = n + ik ) by:
, and (2.18)
ε . (2.19)
Classical Drude theory  can be used for a preliminary analysis of the above relations. Drude theory describes the free electron contribution to the dielectric function by:
(2 2 2
ω ε ω ω γ
+ , and (2.20)
/ ( )
(2 2 2
ω γ ω ω ω γ
+ . (2.21)
is the dielectric constant, and h γ is a relaxation energy which may be taken to be energy independent for qualitative analysis. The electron density and the effective conduction-band mass of the electrons mc*
determine the value of ωN
through the equation:
* 0 2
n e ε m
ω = , (2.22)
F/m is the permittivity of free space. The longitudinal plasma energy h ωp
is approximately related to h ωN
( ω / ε ) γ
− . (2.23)
The values of ε∞
can be determined by plotting ε1
vs , provided that the Drude formalism applies. The plasma resonance frequency
( h ω−
ω is given by:p 2
= π N ε ε∞
ω . (2.24)
The experimental results can be explained well by Drude theory when it is applied to the visible and near-infrared wavelength ranges for ITO films . It is evident that free electrons play a crucial role to determine the optical properties of the films. Due to an inherent limitation of the Drude theory, it is not applicable in the ultraviolet region, because it assumes a constant relaxation time over the whole spectral region, whereas the relaxation time is known to be frequency dependent.
2.3.2 Determination of optical band gap
In the low-wavelength region, the value of optical band-gap can be estimated by the standard relations . The variation of the imaginary part of the dielectric constant
) 2 (2
ε = nk
ε with photon energy for direct allowed band-to-band transition is of the form:
2 / 1 0
( h ν ε = ε h ν − ∆ E , for h ν > ∆ E (2.25)
ε , for h ν < ∆ E (2.26)
where h is the photon energy, ν ε0
is approximately independent of photon energy and
∆ E is the band-gap. The curve (h2
versus h extrapolated to zero gives the value ν of ∆ E .
For allowed indirect transitions, i.e. non-vertical transitions, the imaginary part of the dielectric constant ε2
for a single photon process is given by:
) 1 (
p KT g